Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

1,335 views

Published on

No Downloads

Total views

1,335

On SlideShare

0

From Embeds

0

Number of Embeds

5

Shares

0

Downloads

0

Comments

0

Likes

1

No embeds

No notes for slide

- 1. X-Rays and X-Ray Diffraction 3 3.1 Generation and Properties of X-Rays X-rays are an electromagnetic radiation of short wavelength, and can be produced by the sudden deceleration of rapidly moving electrons at a target material. If an electron falls through a potential difference of V volt, it acquires an energy eV electron-volt (eV), where e is the charge on an electron. This energy may be expressed as quanta of X-rays of wavelength l, where each quantum is given by l ¼ hc=ðeVÞ (3.1) h being the Planck constant and c the speed of light in vacuum. Substitution of numerical values into (3.1) leads to l ¼ 12:4=V (3.2) where V is measured in kilovolt and l is given in Angstrom units (A˚ ). The wavelength range of X-rays is approximately 0.1–100 A˚ , but for the purposes of practical X-ray crystallography, the range used is restricted to 0.7–2.5 A˚ . 3.1.1 X-Rays and White Radiation Except for synchrotron radiation, which is discussed in Sect. 3.1.6, a widely used source of X-rays in conventional crystallography laboratories is the sealed hot-cathode tube with a rotating anode, illustrated diagrammatically in Fig. 3.1. Electrons are emitted from a heated tungsten ﬁlament, the cathode, and accelerated by a high voltage, 40 kV or more, towards a water-cooled target anode, usually made of copper or molybdenum. A large proportion of the energy reaching the target is dissipated as heat on account of multiple collisions within the target material, but about 10% of it is converted usefully for X-ray crystallographic purposes. In order to dissipate the heat rapidly and efﬁciently, the water-cooled anode is rotated, as indicated in the diagram of Fig. 3.1. M. Ladd and R. Palmer, Structure Determination by X-ray Crystallography: Analysis by X-rays and Neutrons, DOI 10.1007/978-1-4614-3954-7_3, # Springer Science+Business Media New York 2013 111
- 2. As a consequence, a higher accelerating voltage can be applied to the tube, which results in a more powerful X-ray source. If the energy eV is not too high, there will be a continuous distribution of X-ray wavelengths, “white” radiation, or Bremsstrahlung (Ger. ¼ braking radiation), as shown in Fig. 3.2. With an increase in the accelerating voltage V, the intensity of the radiation increases, and the maximum of the curve moves to shorter wavelengths. Fig. 3.1 Schematic diagram of a sealed crystallographic X-ray tube. The target anode is provided with a means of rotation, so as to aid the dissipation of heat generated by the electron impact on the target and to prolong the life of the target 112 3 X-Rays and X-Ray Diffraction
- 3. 3.1.2 Characteristic Radiation At a particular higher value of V, the impinging electrons excite inner electrons in the target atoms. Other electrons from higher energy levels then fall back to the inner levels, and their transitions are accompanied by the emission of X-radiation of high intensity, characteristic of the material of the target. The X-ray wavelength depends on the energies of the two levels involved, E1 and E2, such that l ¼ hc=jE2 À E1j (3.3) Figure 3.3 illustrates the curve of radiation intensity against X-ray wavelength, when the accel- erating voltage is sufﬁcient to excite the K spectrum of the target metal. The K spectrum consists of the Ka and Kb wavelengths, which are always produced together, and correspond to electrons falling back to the K level from the L and M levels respectively. Two slightly different L energy levels exist, so that the important Ka spectrum consists of two components, Ka1 and Ka2, of closely similar wavelength. Similarly, M ! K transitions give rise to Kb characteristic radiation. The wavelengths of the K radiations for a target material of copper are: Kb1 ¼ 1.39222 A˚ , Kb2 ¼ 1.38109 A˚ , Ka1 ¼ 1.54056 A˚ , and Ka2 ¼ 1.54439 A˚ . The mean value for Ka is obtained by averaging the Ka1 and Ka2 wavelengths in their intensity ratio of 2:1, thus giving the average value of 1.54184 A˚ for Ka. The a1, a2 doublet is resolved when the angle of scatter is large, that is, at high values of the Bragg angle y (q.v.). Fig. 3.2 Variation of intensity with wavelength for an X-ray tube, for three different operating voltages; as V increases, the maximum wavelength in the continuous spectrum moves to shorter wavelengths, in accordance with (3.2) 3.1 Generation and Properties of X-Rays 113
- 4. 3.1.3 Absorption of X-Rays All materials absorb X-rays, and the transmitted intensity is attenuated according to an exponential law: I ¼ I0 expðÀmtÞ (3.4) I0 and I are, respectively, the incident and transmitted intensities, m is the linear absorption coefﬁcient of the material, and t is the path length for X-rays through the material. The absorption of X-rays increases with the atomic numbers of the elements in the absorbing material. The variation of m with wavelength is illustrated in Fig. 3.4, which refers to elemental nickel. The absorption coefﬁcient m of any material decreases approximately as l5/2 , so that as l falls, the energy of the radiation (hc/l) becomes greater and more penetrating. With continuing decrease in wave- length, a position is reached where the energy of the radiation is sufﬁcient to eject an electron from the L energy level of an atom of the material. At this point, known as the absorption edge, or resonance level, the value of m is greatly enhanced. As the wavelength decreases further, the absorption coefﬁcient continues to fall off as before. In the case of nickel, this particular L absorption edge occurs at a wavelength of 1.4886 A˚ . Absorption edges are important in selecting the correct radiation for a particular application. For example, copper X-radiation would be unsuitable for materials containing a high percentage of iron. The K absorption edge for iron is 1.7433 A˚ , so that radiation of this wavelength would be strongly absorbed by the iron moiety and subsequently re-emitted as the characteristic K spectrum of iron. In such a case, molybdenum radiation, l(Ka) ¼ 0.71073 A˚ , would be a satisfactory alternative. Fig. 3.3 Characteristic K spectrum from an X-ray tube superimposed upon the “white” radiation, or continuous spectrum 114 3 X-Rays and X-Ray Diffraction
- 5. If a material consists of a single elemental species, m in (3.4) may be termed the atomic absorption coefﬁcient [1] ma, given by ma ¼ Mrm=ðDmLÞ (3.5) where Mr is the relative atomic mass, Dm the density of the material, and L the Avogadro constant. Of more general applicability is the mass absorption coefﬁcient mm, given by mm ¼ m/Dm, so that ma ¼ mm(Mr/L). For a compound. we have m ¼ X i mm;iDm;i (3.6) where mm,i is the mass absorption coefﬁcient for the ith species of partial density Dm,i in the compound; Dm,i is calculated for the ith species as Dm;iMm;i=Mr. For example, sodium chloride, NaCl, has a density of 2165 kg mÀ3 , and the relative atomic masses and mass absorption coefﬁcients for Na and Cl are 22.98 and 3.01 m2 kgÀ1 , and 35.45 m2 kgÀ1 and 10.6 m2 kgÀ1 for Na and Cl, respectively. Hence, the linear absorption coefﬁcient for NaCl is given by m ¼ 2165½ð3:01 Â 22:98=58:43Þ þ ð10:6 Â 35:45=58:43Þ ¼ 1:65 Â 104 mÀ1 and this parameter is needed in the correction of X-ray intensities, Sect. 4.1.3. The attenuation factor I/I0, for a crystal of NaCl of thickness 0.1 mm in the path of the X-ray beam, is then exp(À1.65 Â 104 Â 0.1 Â 10À3 ), or 0.192. Fig. 3.4 Variation with wavelength of the linear absorption coefﬁcient m for nickel; the discontinuity at approximately 1.4886 A˚ corresponds with the L absorption edge of the element 3.1 Generation and Properties of X-Rays 115
- 6. 3.1.4 Monochromatic Radiation Usually X-ray structure analysis requires monochromatic radiation, but Figs. 3.2 and 3.3 show that X-ray sources contain a range of wavelengths. However, and in particular for radiation from a copper target, we note that the absorption edge for nickel (1.4886 A˚ ) lies between the wavelengths for Cu Ka and Cu Kb radiations. The effect of passing the X-rays from a copper target through a nickel foil of ca. 0.018 mm thickness is shown in Fig. 3.5, a superposition of Figs. 3.3 and 3.4. The Kb radiation is almost totally absorbed by the nickel, and the “white” radiation is decreased signiﬁcantly in intensity. There is also a loss in intensity of the Ka radiation, but the intense part of the beam behaves as a closely monochromatic, or ﬁltered, radiation. Evidence for a residual presence of Kb and white radiation may be seen in Fig. 9.5 as weak reﬂections just below the strong reﬂections, that is, at lesser y values; the very strong reﬂections also show spots from tungsten La radiation at still lower y values (lLa ¼ 1.476 A˚ ). A similar degree of monochromatization can be obtained with molybdenum radiation if a ﬁlter of zirconium foil is used. Crystals themselves can act as monochromators through application of the Bragg equation (q.v.); we consider this topic in Sect. 5.8.1ff. 3.1.5 Collimation A collimator is used to deﬁne the angular limit of the X-ray beam. The simplest collimator is the pinhole type, a cylindrical device in which the beam is limited usually by two deﬁning circular apertures together with a guard aperture. The collimation provided is satisfactory in many situations, and a divergence angle of approximately 0.02 rad is typical. Figure 3.6a illustrates an elegant apparatus for taking a back-reﬂection Laue photograph of a metal casting, showing also the type of collimator just described. Fig. 3.5 Diagrammatic superposition of the curves of Figs. 3.3 and 3.4, for Cu Ka X-radiation; the strongly preferential absorption of the Kb radiation results in an almost monochromatic Ka radiation 116 3 X-Rays and X-Ray Diffraction
- 7. Improved collimators have been described [2] in which monochromatic X-rays, obtained by crystal reﬂection, are guided by multiple reﬂections within thin-walled borosilicate glass capillary tubes (Fig. 3.6b). It is necessary for the X-rays to be reﬂected from the tube walls at less than the critical angle yc: yc=mrad ¼ 30=V where the voltage V is measured in keV. The divergence at input could be 60–120 mrad, or 5–10 , and 2–4 mrad at output. The system allows a useful X-ray ﬂux from Cu Ka radiation to be produced that is four to ﬁve times stronger than that obtained by simple pinhole collimation, with comparable initial divergence, and the output beam produces uniform diffraction peaks while the higher energy Bremsstrahlung and background radiations are insigniﬁcant. Fig. 3.6 Collimation of X-rays. (a) Colli- mator employed in a back-reﬂection Laue experiment (courtesy of Jackson Electron- ics Newark, UK) (b) Cross-section of a multifiber polycapillary fiber collimator, with about 400 50 m diameter channels (Gibson D, Gibson W (2002) Adv X-ray Anal 45; reproduced by permission of ICDD) 3.1 Generation and Properties of X-Rays 117
- 8. 3.1.6 Synchrotron Sources A synchrotron is a large-scale particle accelerator designed primarily as a tool for fundamental studies in particle physics. However, it has many applications, and in X-ray crystallography it functions as a very powerful source of X-rays, with an intensity of several orders of magnitude greater than that of the sealed X-ray tube. It can generate brilliant beams of electromagnetic radiation from infra-red to X-ray wavelengths. The Diamond Synchrotron Source Figure 3.7 is a schematic diagram of the Diamond synchrotron that was opened at Harwell Science and Innovation Campus in 2007. It consists of several elements, as follow: • In the injection system (1), an electron gun produces a series of pulses of electrons with an energy of approximately 90 keV. These electrons are then accelerated in the linear accelerator LINAC, which raises their energy to about 100 MeV. • The 100 MeV electrons are further accelerated in the booster synchrotron (2). Thirty-six dipole bending magnets of ﬁeld up to 0.8 T are used to curve the electron beam around the bends in the ring, and then they are ejected from the booster with energy of 3 GeV. • The storage ring (3) contains 48 bending magnets that curve the electron beam between the straight sections. The total deﬂection is 360 and the length of the orbit is 561.6 m. The ring is under vacuum, and the 3 GeV electrons complete each circuit in 1.9 Â 10À6 s, thus traveling at 98.6% of the speed of light. • Each beamline (4) comprises three main sections: an optics hutch, an experimental hutch that houses experimental equipment, and a control hutch, and is designed for a speciﬁc experimental application. • The front end (5) channels the synchrotron light into a beamline. It monitors the beam in passing through to the optics hutch. • The optics hutch (6) contains mirrors and diffraction gratings or crystals, the purpose of which is to ﬁlter the beam so as to obtain the desired radiation wavelength, and also to focus it on to the sample under investigation. • The experimental hutch (7) houses the technical equipment for carrying out the experiments and provides a number of different specialized X-ray detectors for the various kinds of experiments. Fig. 3.7 Schematic illustration of the Diamond synchrotron facility at Harwell; the numbered sections are described in the text (reproduced by courtesy of the Diamond Light Source, Harwell Science and Innovation Campus) 118 3 X-Rays and X-Ray Diffraction
- 9. • The control hutch (8) provides the operators with a computer-controlled monitoring system for the experiment in progress. • A radiofrequency cavity in the region of (9) contains an electromagnetic ﬁeld that makes up for the energy that the electrons lose in the form of synchrotron radiation as they travel around the ring. There is also Diamond House, which provides for Diamond staff accommodation, meeting, and conference rooms, and also access to the synchrotron facility itself. The Diamond IO2 beamline, which is concerned with macromolecular X-ray crystallography, has a ﬂux of about 1.5 Â 1012 photon sÀ1 and, typically, an operating wavelength of 0.98 A˚ , giving a resolution of 1.09 A˚ . Beamlines IO3 and IO4 are similar to IO2, and beamlines IO4-1 and I24 are available for microfocus macromolecular crystallography. A fascinating video-description of a trip around the Diamond ring may be found at a web site [3]. Polarization of Synchrotron Radiation An important difference between X-radiation from sealed tube or rotating anode sources and X-rays produced by a synchrotron is their physical state of polarization; see also Sect. 3.2.4. X-rays generated from conventional laboratory sources are totally non-polarized unless a crystal monochromator is employed. In contrast, synchrotron radiation is 100% linearly polarized in the plane of the electron beam orbit and elliptically polarized above and below the plane. In addition, the output radiation is pulsed, because the electrons do not form a uniform stream. Figure 3.8a considers a three-dimensional X-ray wave at the origin, with components of oscillation vibrating in the y and z directions. The beam from a synchrotron is plane-polarized, with the component in the z direction being an order of magnitude less in intensity. X-ray beams from crystal monochromators, because they have undergone Bragg diffraction, are also polarized, but the extent is considerably less. The effect of this primary or beam polarization of synchrotron radiation on the intensity of the diffraction pattern must be taken into account during data processing. This is achieved through application of a polarization factor P that includes a source-dependent property, with components normal and parallel to the plane of polarization: P ¼ ðIk À I?Þ=ðIk þ I?Þ where Ik and I⊥ are the intensities of the electrical ﬁelds of the X-ray beam along and normal to the axis of a rotation camera, respectively. The value of P is calibrated for each workstation at a synchrotron installation. For the Diamond station, P is approximately 0.8, whereas for a graphite monochromator, P is equal to 0.11. A typical synchrotron radiation spectrum is shown in Fig. 3.8b and may be compared with that from the sealed tube. The photon intensity is given in units of photon per second for a horizontal angular aperture of 1 mrad (3.4 min of arc), with a 1 A beam current and a 0.1% spectral bandwidth, after performing vertical integration over the full angular divergence of the radiation above and below the orbital plane. The ﬂux attainable in practice depends upon the multiplying factors set by the values of the dependent parameters. A horizontal aperture of an experimental workstation may be less than 1 mrad for topography, typically 5–10 mrad for the majority of spectroscopy experiments, and up to 40 mrad for the high-aperture port used for time-resolved measurements. The ﬂux available will change proportionally if this resolution is varied. The stored current and, hence the photo ﬂux, gradually decline as electrons are lost by scattering from closed electron orbits. The beam lifetime, that is, the time of fall to approximately 1/e of the initial intensity, is approximately 8 h. 3.1 Generation and Properties of X-Rays 119
- 10. Insertion Devices: Wigglers and Undulators The output characteristics of the synchrotron can be modiﬁed by devices inserted into the straight sections between the magnets. An insertion device is an array of magnets which can be inserted into the straight sections of the storage ring and cause the electron beam to follow a wiggling or undulating Fig. 3.8 (a) A three- dimensional wave traversing the origin, with oscillatory components vibrating along the x and y directions: (i) Conventional X-ray tube radiation, (ii) Synchrotron radiation (not to scale). The radiation from a synchrotron is plane-polarized, with the z component an order of magnitude less than that in the y direction. The spread of radiation in the vertical (z) direction is given as D ¼ mec2 /E, where E is the electron beam energy. (b) Spectral curves in the X-ray region from a normal bending magnet and a wiggler for a 2 GeV 1 A beam in the synchrotron radiation source, and the types of experiment used in the wavelength regions speciﬁed. The peak of the curve is approximately 1.4lc, corresponding to the maximum output of energy per unit wavelength; lc is the critical wavelength for the synchrotron 120 3 X-Rays and X-Ray Diffraction
- 11. path, so as to produce more intense, tuneable light. Insertion devices come in two main types: wigglers and undulators. A wiggler is an insertion device that consists of an array of dipolar magnets of alternating polarity which cause the electron beam to follow a wiggling path of oscillations perpendicular to its general direction. This causes the light to be produced in a wide cone, spanning a broad spectrum of X-rays. Wigglers are used in beamlines where the priority is for very high energy X-rays. An undulator, which is more common at the Diamond installation, is an insertion device that produces a very bright light in a very narrow beam. By varying the separation of the magnet arrays, it is possible to tune the undulator and choose the energy that is generated. They can be used to produce very high energy X-rays over a continuous frequency range, which is essential for many experiments, particularly in protein crystallography. The synchrotron source may be said to have revolutionized X-ray crystallography in certain applications. It has enabled a rapid collection of data to be achieved, and so is of great value in dealing with relatively unstable crystals, such as proteins, with poorly diffracting specimens or polymers, in time-resolved studies, or in solid-state reactions and other transformations, including enzyme-catalyzed processes, or in X-ray topographical studies of crystal defects. Laser-Wakeﬁeld Acceleration Relatively recent work on synchrotron sources has concentrated on a reduction in the physical size of the accelerator. If a high-powered, femtosecond (10À15 s) laser pulse is focused into a plasma, an electrostatic wake is produced which can be harnessed to accelerate electrons to GeV energies within centimeter distances. Electrons become separated from the positive ions, and a ponderomotive force, which is a non-linear force that a charged particle experiences in an inhomogeneous oscillating electromagnetic ﬁeld, arising from the laser light pushes aside the plasma electrons so as to create a wake from the plasma. The associated electrostatic ﬁelds can produce an accelerating ﬁeld of three to four orders of magnitude greater than in the conventional accelerator. In one application of the procedure [4], a laser pulse of 37 fs is ﬁred at a cell of hydrogen gas atoms, thus energizing the electrons and causing them to break free. The positive attraction of the nucleus acts to retain the electrons and the result is an oscillation about the nucleus that produces a plasma wave in the cell. This excitation is similar to the water-wave behind a motorboat; hence, the term wake-ﬁeld (or wakeﬁeld). Other electrons “ride” this wave at relativistic speeds and so generate X-rays through their oscillatory changes. An important feature in the process is the use of a miniature undulator. The combination of a 1.5 cm accelerator and a 30 cm magnetic undulator produced electron energies of 210 MeV. Further research aims at higher electron energies, so that laser-wakeﬁeld acceleration can generate X-rays in the useful wavelength range for diffraction experiments, and with facilities of centimeter size. This development has great potential for X-ray studies on proteins and viruses, where powerful X-ray sources are desirable, because of the low stability of some of these compounds. 3.2 X-Ray Scattering Scattering occurs generally when electromagnetic radiation interacts with matter. Two everyday examples of scattering are the blue color of the sky and the haloes around distant car lights at night that arise from Rayleigh scattering, a highly wavelength-dependent elastic scattering of the light by gas molecules or dust particles in the air. The pattern seen when looking at a sodium street-lamp through a stretched handkerchief or an umbrella, which are approximately two-dimensional net structures, shows an aspect of diffraction similar to that which we shall be discussing with X-rays 3.2 X-Ray Scattering 121
- 12. and crystals, namely the interaction of radiation with a periodic distribution of matter. The X-ray scattering from a crystal is described in terms of the intensity of the scattering function and the angle of scatter. 3.2.1 Scattering by a Single Electron If a plane monochromatic X-ray beam of wavelength l is incident upon an electron at an origin O, then the amplitude C2y of the scattered beam at a point P in the forward direction at unit distance from the origin is given by [5] C2y ¼ f2yC0 (3.7) where C0 is the amplitude of the incident wave, 2y is the scattering angle, and f2y is a constant of proportionality that we shall discuss more fully shortly. 3.2.2 Scattering by Two or More Electrons Let a second electron be introduced at a point A, Fig. 3.9. We need now to determine the phase difference at any point P in the forward direction, where OP is much greater than OA, for the wavelets scattered by the two electrons. The path difference d between the two wavelets scattered by O and A is OY À AX; thus the phase difference f is (2p/l)d, that is, f ¼ ð2p=lÞðOY À AXÞ (3.8) If the distance OA is jrj, then the incident and diffracted waves may be deﬁned by the unit vectors s0 and s, respectively, such that AX ¼ r·s0 and OY ¼ r·s. Thus, f ¼ 2pðr Á s À r Á s0Þ=l ¼ 2pr Á ðs=l À s0=lÞ ¼ 2pr Á S (3.9) From Fig. 3.10, it is clear that S is a vector normal to a plane through O that may be regarded conveniently as a reﬂecting plane; hence, S ¼ js À s0j=l (3.10) so that the magnitude jSj, or S, is equal to 2 sin y=l. Fig. 3.9 Combined scattering at two centers O and A; s0 and s are unit vectors in the incident and scattered beams, respectively; dv is a small volume element at A. 122 3 X-Rays and X-Ray Diffraction
- 13. The amplitude of the wave scattered at P by the two electrons is thus C2y ¼ f2y þ f2y expði2pr Á SÞ ¼ f2y½1 þ expði2pr Á SÞ (3.11) The use of the exponential term to represent relative phase is explained below in Sect. 3.2.3 on the Argand Diagram. In the case that neither of the electrons of the previous example occupies the origin, so there is no zero relative phase involved, then the number 1 on the right-hand side of (3.11) would be replaced by another exponential term. In general, the result for n electrons is given by C2y;n ¼ f2y Xn j¼1 expði2prj Á SÞ (3.12) This equation assumes that the n scattering species have equal power, which would be true if they were all electrons, or identical atoms. In the event that the scattering species are unequal, then the function f2y would be unique to each species and included within the summation as f2y,j. The scattering process itself introduces a phase shift with respect to the origin, but this applies equally to all atoms and may be ignored for our purposes. 3.2.3 Waves and Wave Sums In (3.12), we considered the summation of waves of equal scattering power. In general, each scattering entity will be allocated its own scattering function and phase. Each wave then takes the form fj exp(ifj), where fj ¼ rj Á S. For convenience, we may drop the subscript y (or 2y) to f ; unless we speciﬁcally want to emphasize its dependence on y; we know that such dependence is always present. Using de Moivre’s theorem, the exponential term may be expanded into cosine (real) and sine (imaginary) components: expðÆifÞ ¼ cos fÆ i sin f, and a straightforward way of representing a wave is in the complex plane of an Argand diagram. Fig. 3.10 Relationship of the scattering vector S, or (s À s0)/l, to the reﬂecting plane (hkl). The vector S is normal to the plane (hkl), and its magnitude jSj, or S, is 2 sin y=l 3.2 X-Ray Scattering 123
- 14. Argand Diagram In Fig. 3.11, we show the combination of two waves of scattering factors f1 and f2 on an Argand diagram to give a resultant F, which we shall later identify with the structure factor, Sect. 3.5.1: F ¼ f1 expðif1Þ þ f2 expðif2Þ (3.13) F is a scalar quantity but may be manipulated like a vector in the complex plane, having both a magnitude and direction; exp(if) may be regarded as an operator that rotates f counterclockwise on an Argand diagram by the angle f measured from the positive, real axis. The foregoing analysis may be extended to n waves. The resultant sum F is, from (3.13), F ¼ f1 expðif1Þ þ f2 expðif2Þ þ Á Á Á þ fj expðifjÞ þ Á Á Á ¼ Xn j¼1 fj expðifjÞ (3.14) The Argand diagram, Fig. 3.12, expresses (3.14) as a polygon of f-“vectors” for the combination of six waves, and the resultant F may be expressed as F ¼ jFj expðifÞ (3.15) where the amplitude jFj is obtained from jFj ¼ ðFFÃ Þ1=2 (3.16) F* is the complex conjugate of F, that is, jFj expðÀifÞ, Fig. 3.13. Resolving the resultant F of the six waves into its real and imaginary components, we have Fig. 3.11 Combination of the two waves f1 exp(if1) and f2 exp(if2), shown as vectors on an Argand diagram. The resultant is F, and its phase is expressed by the angle f between F and the R (real) axis 124 3 X-Rays and X-Ray Diffraction
- 15. Fig. 3.12 Combination of six waves on an Argand diagram: F ¼ P6 j¼1 fj expðifjÞ Fig. 3.13 The quantity F(hkl) for a reﬂection from an (hkl) family of planes and its components A0 (hkl) and B0 (hkl); f(hkl) is the phase angle for F(hkl). The conjugate F* (hkl), or Fðh k lÞ, has the same magnitude for A0 and B0 , but the sign of B0 is reversed; hence fðhklÞ ¼ Àfðh k lÞ. In a centrosymmetric structure, F(hkl) lies along the real axis, so that F (hkl) ¼ A0 (hkl), or F(hkl), and its phase is either 0 or p. Then, since A0 (hkl) ¼ jF(hkl)j cos f, it is common to speak of the sign of F(hkl), that is, ÆF(hkl), in a centrosymmetric structure 3.2 X-Ray Scattering 125
- 16. jFj ¼ ðA02 þ B02 Þ1=2 (3.17) where A0 ¼ Xn j¼1 fj cos fj (3.18) and B0 ¼ Xn j¼1 fj sin fj (3.19) The phase f of the resultant F is given by f ¼ tanÀ1 ðB0 =A0 Þ (3.20) Graphical Representation of Wave Sums When waves of equal frequency, those in which we are interested, combine, the resultant can be determined through (3.17–3.20). If two waves are in exact register—path difference, nl—the resultant amplitude is simply the sum of the individual amplitudes. If the waves are exactly out of phase—path difference, (n + 1)l/2—the resultant is the difference between the amplitudes. All cases between these extremes are possible, depending on the values of the amplitudes jFj and phase angles f. In Fig. 3.14, we represent the combination of two waves, one of amplitude 100 (f1) and phase 0 , and the other of amplitude 50 (f2) and phase 240 , with respect to the origin. From the foregoing, the amplitude of the resultant becomes jFj ¼ ½ðf1 cos f1 þ f2 cos f2Þ2 þ ðf1 sin f1 þ f2 sin f2Þ2 1=2 (3.21) and the phase of the resultant is f ¼ tanÀ1 ½ðf1 sin f1 þ f2 sin f2Þ=ðf1 cos f1 þ f2 cos f2Þ (3.22) Importance of Correct Phases As shown in the legend to Fig. 3.14, the resultant amplitude jFj is 86.6 and its phase f is 330 . From the ﬁgure we can see the importance of the correct phase of a wave (reﬂection). The peaks (atomic positions) in this ﬁgure occur at 330 Æ 2p (Æ360 ). If, on one hand, we decrease f2 to 25, the resultant amplitude is 90.1, because the sine term subtracts a smaller amount, and the phase is 346 , a small change in position. If on the other hand, we decrease the phase by half, leaving f2 unchanged, then the resultant amplitude is again 86.6, but the phase (atomic position) is now at +30 , a very different situation; see Problem 7.11. 126 3 X-Rays and X-Ray Diffraction
- 17. 3.2.4 Coherent and Incoherent Scattering Coherent (Thomson) Scattering: Polarization In coherent scattering, the incident and scattered waves have the same wavelength, and there is a deﬁnite phase relationship between the incident and scattered radiations. When X-rays fall upon an electron, the alternating electric-ﬁeld vector imparts an alternating acceleration to the electron. Classical electromag- netic wave theory shows that an accelerated charged particle emits radiation, through a process of absorption and re-emission, the emitted radiation traveling in all directions for a given angle of scatter. A theoretical treatment of Thomson scattering [5] shows that the intensity I2y of the scattered radiation of incident intensity I0, deﬁned as power per unit solid angle, is I2y ¼ 1 2 ½e2 =ð4pe0c2 meÞ2 ð1 þ cos2 2yÞI0 (3.23) Fig. 3.14 Combination of two waves of amplitudes 100 (f1) and 50 (f2) with phases 0 (f1) and 240 (f2), respectively. The resultant wave has an amplitude jFj and a phase f. (a) First wave. (b) Second wave. (c) Resultant wave F, given by ¼ [(100 + 50 cos 240)2 + (50 sin 240)2 ]1/2 ¼ 86.6; f ¼ tanÀ1 [(50 sin 240)/(100 + 50 cos 240)] ¼ À30 (330 ) 3.2 X-Ray Scattering 127
- 18. where e is the charge on an electron, e0 is the permittivity of a vacuum, c is the speed of light in a vacuum, and me is the mass of the electron. The factor 1=me shows how electrons are the only effective scattering species for X-rays: even the lightest species, hydrogen, although it has the same magnitude of charge, is ca. 1,840 times heavier than the electron. This result shows also that neutrons are excluded from the category of X-ray scattering species because they are uncharged particles. The term 1 2 ð1 þ cos2 2yÞ is a geometrical factor known as the polarization factor p for X-ray scattering, which we shall encounter further in ensuing chapters. p ¼ 1 2 ð1 þ cos2 2yÞ (3.24) Incoherent (Compton) Scattering With incoherent scattering, the wavelength of the scattered radiation is longer than that of the incident radiation, which implies a loss of energy in the scattering process, owing to elastic collisions of electrons with photons. An analysis [5] shows that in Compton scattering, the wavelength change dl is given by dl ¼ ½h=ðmecÞð1 À cos 2yÞ (3.25) or, by inserting the fundamental constants in appropriate units, dl ðA) ¼ 0:0243ð1 À cos 2yÞ (3.26) Thomson scattering illustrates the particle property of the electron, whereas Compton scattering shows its wave nature. 3.2.5 Scattering by an Atom In an atom, electrons are bound in levels of distinct energies, and in the scattering of X-rays by an atom both coherent and incoherent scattering are involved. A full analysis of the scattering process requires a wave-mechanical treatment, involving both modes of scattering, from which we obtain the electron density function r, where r ¼ CC* and C* is conjugate to C; if we assume a real nature for the electron density function then r ¼ jCj2 , and the expression may be interpreted such that C2 dt, or r dt, represents the probability of ﬁnding the electron in a volume element dt. We shall use the Thomson formula only because incoherent scattering contributes to the background radiation and is but a small fraction of the total intensity in the case of crystalline materials. Consider a plane of atoms in a crystal. We demonstrate in the ensuing sections that all atoms on this plane scatter in phase with one another and with the atoms in parallel planes, for a given scattering vector S. Thus, we need to consider how the electrons in any one atom combine in order to obtain the total scattering amplitude for the atom. Let rðrÞ dt be the probability that an electron in the chosen atom lies in a small volume element dt distant r from the origin, the center of the atom, where r is the magnitude of the vector r, as shown in Fig. 3.15. If f(S) represents the scattering power of the atom in the direction S, then we have from the foregoing: fðSÞ ¼ ð rðrÞ expði2pr Á SÞ dt (3.27) 128 3 X-Rays and X-Ray Diffraction
- 19. Let S make an angle C with the direction of r. Then 2pr Á S ¼ ð4p=lÞ sin y r cos C ¼ mr cos C where m ¼ 4p(sin y)/l. Since spherical symmetry has been assumed, the volume element dt is a spherical annulus of radius r and thickness dr on S as axis, so that dt ¼ 2pr2 dC dr. Let mr cos C ¼ x, so that dx ¼ Àmr sin C dC. Now (3.27) may be expressed as fðSÞ ¼ 2p ð1 0 r2 rðrÞ=mr dr ðÀmr mr À expðixÞ dx ¼ 4p ð1 0 r2 rðrÞðsin mrÞ mr dr= (3.28) Since m ¼ (4p sin y)/l, (3.28) may be recast as a function of jSj: fðSÞ ¼ 4p ð1 0 r2 rðrÞðsin 2prSÞ ð2prSÞ= dr (3.29) where S is 2 sin y=l. The atomic scattering factor may be deﬁned as the ratio of the amplitude of coherent scattering from an atom to that scattering by a single electron at the center of the atom. It follows from (3.29) that, for scattering in the forward direction, when (sin 2prS)/(2prS) ¼ 1, the expression Ð1 0 r2 rðrÞ dr becomes the total electron density for the atom. Hence, we may write fðSÞS¼0 ¼ Z (3.30) Fig. 3.15 Scattering by a single atom. A section of a sphere of radius r, showing an annular ring of thickness dr at an angle C to the scattering vector S. The volume of the annular ring is ½pðr þ drÞ2 À pr2 r sin C dC ¼ 2pr2 sin C dC dr (neglecting second order terms in dr) 3.2 X-Ray Scattering 129
- 20. where Z is the total number of electrons in the atom, or atomic number; S ¼ 0 is equivalent to sin y ¼ 0 in terms of the y-angle. As an example calculation, we consider the contribution of a 1s electron to f(S). We equate r(r) to jC1sj2 and use Slater’s analytical wavefunctions. The Slater one-electron 1s wavefunction C1s may be written as ð1= ﬃﬃﬃ p p Þc 3=2 1 expðÀc1=rÞ; c1 is (Z À s)/a0, where s is Slater’s quantum mechanical screening constant [6] and a0 is the Bohr radius for hydrogen. With lithium, for example, s1s ¼ 0.30 and, remembering that r / C2 , we have from (3.29), f1sðSÞ ¼ 2c3 1=ðpSÞ ð1 0 r expðÀc1rÞ sinð2pSrÞ dr From a table of standard integrals, or by use of the G function (see Web Appendix WA7), ð1 0 x expðÀaxÞ sinðbxÞ dx ¼ 2ab=ða2 þ b2 Þ 2 so that f1sðSÞ ¼ c4 1=ðc2 1 þ p2 S2 Þ2 (3.31) In lithium, for example, there are two contributions from (3.31) and one contribution from a similar expression for the 2s electron (see also Problem 3.3). They are added to obtain the value of f at a given value of S. Atomic scattering factor data are readily available, quoted normally as functions of sin y=l. Such data refer to systems of electrons at rest: at a ﬁnite temperature, the effective scattering from an atom is less than the value at rest, and we shall discuss this situation later in this chapter. A satisfactory calculation of rest atomic scattering factors is afforded by the equation fðsÞ ¼ X4 j¼1 aj expðÀbjs2 Þ þ cj (3.32) where s is sin y=l, and the nine constants required by the equation have been recorded for all atomic and some ionic species [7]. 3.3 Scattering by Regular Arrays of Atoms The interaction of X-rays with a crystal is a complex process, often described as a diffraction phenomenon although, strictly speaking, it is a combined scattering and interference effect. Two treatments, those of von Laue and Bragg, describe the process, and we shall consider them in that order. 3.3.1 Laue Equations Figure 3.16 represents a regular, one-dimensional array of atoms of spacing b, imagined in three- dimensional space. Parallel X-rays are incident at an angle f2 and scattered at an angle C2 to the direction of b. The path difference for rays scattered by neighboring centers is represented by 130 3 X-Rays and X-Ray Diffraction
- 21. AQ À BP, or b(cos C2 À cos f2); this difference must be equal to an integral number of wavelengths for reinforcement to occur, so that bðcos C2 À cos f2Þ ¼ kl ¼ b Á s À b Á s0 (3.33) where s and s0 have meanings as before. This equation may be written alternatively, using (3.10), as b Á ðs À s0Þ=l ¼ b Á S ¼ k (3.34) The generators of a cone of semivertical angle C2, coaxial with the row in Fig. 3.16, satisfy (3.33). For a given value of f2, there will be a series of cones corresponding to the orders of k (k ¼ 0, 1, 2, . . .), as shown in Fig. 3.17. Fig. 3.16 Diffraction from a row of scattering centers, of spacing b along the y axis. The Laue equation b(cos C2 À cos f2) ¼ kl, or b Á S ¼ k, is satisﬁed by any generator of the cone Fig. 3.17 Several orders of diffraction can arise from a row of scattering centers, for a given value of f2, corresponding to integral values for k 3.3 Scattering by Regular Arrays of Atoms 131
- 22. The discussion is extended readily to a net a, b, so giving rise to a second condition a Á ðs À s0Þ=l ¼ a Á S ¼ h (3.35) A second cone now intersects the ﬁrst cone generally in two lines, but for the special case that both (3.34) and (3.35) hold simultaneously, the two lines coincide and the atoms of the net scatter in phase, with the incident and diffracted beams lying in the plane of the net. Generalizing the argument to three dimensions, we obtain the complete Laue equations: a Á S ¼ h b Á S ¼ k c Á S ¼ l (3.36) Any of the three possible pairs of equations deﬁne scattering from the corresponding net, but for the particular case that all three equations apply simultaneously, the three-dimensional array scatters in phase and produces the hkl spectrum. Referring to Fig. 1.12 mutatis mutandis, we can rewrite (3.36) as a Á S ¼ 2a sin y=l cos a ¼ h b Á S ¼ 2b sin y=l cos b ¼ k c Á S ¼ 2c sin y=l cos g ¼ l (3.37) where h, k, and l are integers. The direction cosines cos a, cos b, and cos g of the vector S, normal to the reﬂecting plane, with respect to the directions of a, b, and c are, therefore, proportional to a/h, b/k, and c/l, respectively. Successive planes (hkl) in the crystal intersect the x, y, and z axes at a/h, b/k, and c/l, respectively, so that they are parallel to the reﬂecting plane (hkl). Thus, (3.37) show that a scattered beam may be considered as derived from the incident beam by “reﬂection” from the (hkl) family of planes. Furthermore, if d(hkl) is the interplanar spacing, then from Sect. 1.2.2, dðhklÞ ¼ a=h cos a ¼ b=k cos b ¼ l=c cos g (3.38) and (3.37) shows that 2dðhklÞ sin y ¼ l (3.39) a relation deduced by Bragg, originally in the form 2d(hkl) sin y ¼ nl. 3.3.2 Bragg Equation The deduction of the Bragg equation, sometimes thought to be ad hoc, was occasioned by the observation that if a crystal in a position that produced a scattered X-ray beam was rotated through an angle j to another scattering position, then the scattered beam had been rotated through 2j, as in the reﬂection of light from a plane mirror. In Fig. 3.18, two planes from a family of planes (hkl) are shown, together with the incident and reﬂected rays. The part of the incident beam that is not reﬂected at a given level passes on to be 132 3 X-Rays and X-Ray Diffraction
- 23. reﬂected from a deeper level in the crystal. Furthermore, all rays reﬂected from a given level remain in phase after reﬂection, because there is no path difference between them. The path difference d between the two reﬂected rays shown is given by d ¼ QA2 þ A2R ¼ A1A2 cos f2 ¼ A1A2ðcos f1 þ cos f2Þ ¼ 2A1A2 cos½ðf1 À f2Þ=2 cos½ðf1 þ f2Þ=2 (3.40) which, by simple manipulation, becomes d ¼ 2d sin y (3.41) Since d is independent of f1 and f2, (3.41) applies to all rays in the bundle reﬂected from the adjacent planes. By the usual rules that apply to the combination of waves, the reﬂected rays will interfere with one another, the interference being at least partially destructive unless the path difference d is equal to an integral number of wavelengths. Hence, we obtain the Bragg equation, as originally formulated: 2d sin y ¼ nl (3.42) where n is an integer. The mirror-reﬂection analogy breaks down in practice because this equation must be satisﬁed for a reﬂection to occur, but the treatment is, nevertheless, a very useful geometrical way of looking at the X-ray diffraction process. In (3.42), n is the order of the Bragg reﬂection. From Sect. 2.4, we recall that d(hkl)/n ¼ d(nh, nk, nl), with h, k, and l taking common factors as necessary. Thus, n is included in the deﬁnition of d(hkl), and the Bragg equation now written as 2dðhklÞ sin yðhklÞ ¼ l (3.43) Each reﬂection from a crystal must now be considered, effectively, as ﬁrst-order from the (hkl) family of planes, speciﬁed uniquely by their Miller indices. To illustrate this argument further, Table 3.1 lists data for planes parallel to (120) in a cube of side 5 A˚ . The Bragg and von Laue treatments are equivalent, and we shall use them as the occasion demands. It has been convenient for this discussion, although not necessary, to consider Fig. 3.18 Geometry of X-ray reﬂection. The path difference between the two typical rays reﬂected from successive planes is (QA2 + A2R). When this difference is equal to an integral number of wavelengths l, a reﬂection is obtained, according to the Bragg equation 3.3 Scattering by Regular Arrays of Atoms 133
- 24. that the scattering material is concentrated at lattice points, or on lattice planes. In general, electron density is a continuous function, albeit with a lattice-like distribution in the crystal. 3.3.3 Equivalence of the Laue and Bragg Equations A way of demonstrating the equivalence between the Laue and Bragg treatments is illustrated by Fig. 3.19. Let p be the spacing between adjacent scattering points A and B in any row of a three- dimensional lattice. An X-ray beam makes the incident angle f with the row of points, and C is the angle between the diffracted ray and the same row. A “reﬂecting” plane must be in such a position as to make an angle y with both rays; the dashed line in the ﬁgure is the trace of such a plane. Following Sect. 3.3.1, we write pðcos C À cos fÞ ¼ nl (3.44) where m is an integer. Expanding (3.44), we obtain À 2p sinððC þ jÞ=2Þ sinððC À jÞ=2Þ ¼ nl. It follows from the diagram that f À y ¼ C þ y so that ðf=2Þ ¼ ðC=2Þ þ y, whereupon p sinððC þ fÞ=2Þ ¼ p sinðC þ yÞ ¼ d and ððC À fÞ=2Þ ¼ ðC=2Þ À ððC=2Þ þ yÞ ¼ Ày. Hence, Table 3.1 Nomenclature for interplanar spacings Original Bragg notation Current usage hkl Order d (A˚ ) hkl d (A˚ ) 120 1 2.236 120 2.236 2 2.236 240 1.118 3 2.236 360 0.745 4 2.236 480 0.559 Fig. 3.19 Equivalence of the Laue and Bragg treatments of X-ray diffraction 134 3 X-Rays and X-Ray Diffraction
- 25. 2d sin y ¼ nl (3.45) which is the Bragg equation (3.42) derived above. 3.3.4 Further Analysis of the Path Difference In (3.12) we expressed the resultant wave from n scattering centers, there thought of as electrons. Now, we can consider them as atoms each speciﬁed in scattering power by f(S). The contribution to a wave scattered by the Ath atom in a unit cell is given by fAðSÞ expði2prA Á SÞ, where the exponential term is the phase of the contribution from the Ath atom. Now the distance r from the origin to atom A is expressed through rA ¼ xAa þ yAb þ zAc (3.46) where xA, yA, and zA are the fractional coordinates of atom A, as before. Since jSj ¼ 2 sin yðhklÞ=l, which from (3.43) is 1/d(hkl), or d* (hkl) (taking k as 1), S is the reciprocal lattice vector d* (hkl). Applying (2.15) we have rA Á S ¼ ðxAa þ yAb þ zAcÞ Á ðhaÃ þ kbÃ þ lcÃ Þ ¼ hxA þ kyA þ lzA (3.47) since a Á aÃ ¼ 1, and a Á bÃ ¼ 0, and similarly for b and c. Thus, from (3.12), the phase angle fA for an atomic species A and its phase contribution are now given by 2prA Á S, or fA ¼ 2pðhxA þ kyA þ lzAÞ (3.48) and the phase contribution is, therefore, exp½i2pðhxA þ kyA þ lzAÞ. 3.4 Reciprocal Lattice: Analytical Treatment We considered a geometrical derivation of the reciprocal lattice in Sect. 2.4, as we believe that treatment forms a straightforward introduction to it. Here, we shall discuss the reciprocal lattice in greater detail. In considering the stereographic projection, we showed that the morphology of a crystal could be represented by a bundle of lines, drawn from a point, normal to the faces of the crystal. This description, although angle-true, lacks linear deﬁnition. The representation may be extended by giving each normal a length that is inversely proportional to the corresponding interplanar spacing in real space, and applying it to all possible lattice planes, so forming a reciprocal lattice. Let a Bravais (real-space) lattice be represented by the unit cell vectors a, b, c. The reciprocal lattice unit cell is deﬁned by the vectors a* , b* , c* , such that a* is perpendicular to b and c, and so on. Then, aÃ Á b ¼ aÃ Á c ¼ bÃ Á a ¼ bÃ Á c ¼ cÃ Á a ¼ cÃ Á b ¼ 0 (3.49) The magnitudes of the reciprocal unit cell vectors are deﬁned by aÃ Á a ¼ bÃ Á b ¼ cÃ Á c ¼ k (3.50) 3.4 Reciprocal Lattice: Analytical Treatment 135
- 26. where k is a constant, normally equal to unity in theoretical discussions, and to an X-ray wavelength in practical applications where the size of the reciprocal lattice is important. In Fig. 3.20, the z* (c* ) axis is normal to the plane a, b. Since c Á cÃ ¼ ccÃ cos ﬀCOR, that is, taking k ¼ 1 in this discussion, cÃ ¼ jcÃ j ¼ 1=ðc cos ﬀCORÞ (3.51) the magnitude of c* in reciprocal space is inversely proportional to the c-spacing in real, or Bravais, space; similar deductions can be made for both a* and b* . Since c* is normal to both b and c, it lies in the direction of their vector product: cÃ ¼ ða Â bÞ (3.52) where is a constant. Let V be the unit cell volume in real space. Then, V ¼ c Á ða Â bÞ (3.53) Now a Â b is a vector of magnitude ab sin g, the area of OADB, directed normal to the plane of a, b and forming a right-handed set of directions with a and b. Then, c Á cÃ ¼ c Á ða Â bÞ ¼ V ¼ 1 (3.54) Hence, cÃ ¼ jcÃ j ¼ ðab sin gÞ=V (3.55) with values for a* and b* obtained by cyclic permutation. The angle g* between a* and b* can be obtained by the equations of spherical trigonometry (see Web Appendices WA2 and WA3). From the discussion therein, we derive Fig. 3.20 Triclinic unit cell, showing its vectors a, b, and c, and the corresponding reciprocal unit-cell vectors, a* , b* , and c* 136 3 X-Rays and X-Ray Diffraction
- 27. cos gÃ ¼ ðcos a cos b À cos gÞ= sin a sin b (3.56) with corresponding expressions for a* and b* obtained by cyclic permutation. Simpliﬁed expressions obtain for (3.51)–(3.56) when the crystal symmetry is higher than triclinic. 3.4.1 Reciprocal Lattice Properties In the Web Appendix WA6, we derive a number of useful properties of the reciprocal lattice, and we summarize the results here. Unit-Cell Volumes in Real and Reciprocal Space The volume of the unit cell may be evaluated as follows. From (3.53), and expressing a, b, and c in terms of a set of orthogonal unit vectors, we derive the equation for a unit-cell volume Vc in terms of its six constants, as shown in Web Appendix WA6; thus Vc ¼ abcð1 À cos2 a À cos2 b À cos2 g þ 2 cos a cos b cos gÞ1=2 (3.57) In the same Appendix, we show also that VcVÃ ¼ k (3.58) where V* is the volume of the reciprocal unit cell and k has the meaning as before. Interplanar Spacings From (2.16), the general equation for d* (hkl) is obtained in terms of the reciprocal unit cell constants from jdÃ ðhklÞj2 ¼ ðhaÃ þ kbÃ þ lcÃ Þ Á ðhaÃ þ kbÃ þ lcÃ Þ ¼ h2 aÃ2 þ k2 bÃ2 þ l2 cÃ2 þ 2klbÃ cÃ cos aÃ þ 2lhcÃ aÃ cos bÃ þ 2hkaÃ bÃ cos gÃ (3.59) and so sin2 yðhklÞ ¼ l2 =½4d2 ðhklÞ ¼ l2 dÃ2 ðhklÞ=4 (3.60) Simpliﬁcations of (3.59) arise in the presence of symmetry higher than triclinic and have been detailed adequately in Table 2.4. Angle Between Planes Given any two planes h1k1l1 and h2k2l2, the angle between them can be found as the supplement of the angle between the two normals, d* (h1k1l1) and d* (h2k2l2); this angle is the interfacial angle of the stereographic projection, Sect. 1.3. In general, the angle f between the forward directions of two vectors p and q is given through cos f ¼ ðp Á qÞ=pq (3.61) 3.4 Reciprocal Lattice: Analytical Treatment 137
- 28. Applying (2.16) for the two planes h1k1l1 and h2k2l2, we ﬁnd cos f ¼ ½h1h2aÃ2 þ k1k2bÃ2 þ l1l2cÃ2 þ ðk1l2 þ k2l1ÞbÃ cÃ cos aÃ þ ðl1h2 þ l2h1ÞcÃ aÃ cos bÃ þ ðh1k2 þ h2k1ÞaÃ bÃ cos gÃ =½dÃ ðh1k1l1ÞdÃ ðh2k2l2Þ (3.62) Reciprocity of F and I Unit Cells We show in the Web Appendix WA6 how an F unit cell reciprocates into an I unit cell (and conversely), where the I unit cell is deﬁned by the vectors 2aÃ F; 2bÃ F, and 2cÃ F. If, as is customary in practice, we deﬁne the reciprocal of an I unit cell by vectors aÃ F; bÃ F, and cÃ F, then only those reciprocal lattice points for which each of h + k, k + l (and l + h) is an even integer belong to the reciprocal of the I unit cell. In other words, Bragg reﬂections from an F unit cell have indices of the same parity; see also Sect. 3.7.1 and Table 3.2. 3.4.2 Reciprocal Lattice and Reflection Condition: Ewald Sphere A section of a reciprocal lattice is shown in Fig. 3.21a: the vectors s0/l and s/l lie in the incident and scattered X-ray beams respectively; a crystal is situated at the point C. The vector QP, which is also the direction of S, must be normal to an (hkl) plane and have the magnitude 2 sin y=l. When the conditions for diffraction are satisﬁed, according to (3.43), S ¼ jd* (hkl)j. A sphere of radius 1/l is described on C as center, and passing through Q, the origin of the reciprocal lattice. If another reciprocal lattice point, such as P, lies on the sphere, then a diffracted beam arises and the vector CP is the direction of this beam; the incident beam vector is along CQ. The sphere is known as the sphere of reﬂection, or Ewald sphere [8], and will be required in subsequent chapters. We note that although we always refer to the “Ewald” sphere, the ﬁrst suggestion for this device came from Bernal [9]. Figure 3.21b is an alternative way of looking at the Ewald sphere construction, in this case taking the radius of the sphere as unity, so that reciprocal space has the units of lengthÀ1 . The conclusions from the construction are, of course, the same, as we can see: from the ﬁgure AQ ¼ 2 and ﬀ APQ ¼ 90 , so that QP ¼ AQ sin yðhklÞ, or 2 sin yðhklÞ. From (3.43), 2 sin y ðhklÞ ¼ l=dðhklÞ, and from Sect. 2.4, we may identify the point P with the reciprocal lattice point hkl. Hence, QP ¼ d* (hkl). Since k ¼ l in this construction, dÃ ðhklÞ ¼ 2 sin yðhklÞ. Thus, the reﬂection from the (hkl) Table 3.2 Limiting conditions for centered unit cells Unit-cell-type Limiting conditions Associated translations Structure factor multiplier G P None None 1 A hkl: k + l ¼ 2n b/2 + c/2 2 B hkl: l + h ¼ 2n c/2 + a/2 2 C hkl: h + k ¼ 2n a/2 + b/2 2 I hkl: h + k + l ¼ 2n a/2 + b/2 + c/2 2 F hkl: h + k ¼ 2n a/2 + b/2 4 hkl: k + l ¼ 2n b/2 + c/2 hkl: (l + h ¼ 2n)a c/2 + a/2 Rhex b hkl: Àh + k + l ¼ 3nobv a/3 + 2b/3 + 2c/3 3 2a/3 + b/3 + c/3 or hkl: h À k + l ¼ 3nrev a/3 + 2b/3 + c/3 3 2a/3 + b/3 + 2c/3 a This condition is not independent of the other two b See Sect. 2.2.3 and Table 2.3 138 3 X-Rays and X-Ray Diffraction
- 29. plane occurs when the hkl reciprocal lattice point lies on the sphere of reﬂection, and the direction of reﬂection is, again, that of CP. 3.5 Scattering by a Crystal Structure In Sect. 2.2ff, we discussed the geometrical properties of the lattices on which crystal structures are based and showed how the arrays of atoms or molecules may be arranged according to space-group symmetry. We need next to consider the diffraction of X-rays by a crystal. We refer the process of scattering to a conventional unit cell and determine the resultant effect of all atoms in the unit cell, Fig. 3.21 (a) Sphere of reﬂection, radius 1/l, with the crystal at C, the center. The origin of the reciprocal lattice is at Q. When a reciprocal lattice point, such as P, lies on the Ewald sphere, a reﬂection arises along the direction CP. (b) Alternative, equivalent picture, but with the sphere of radius 1 (dimensionless), showing the position of crystal planes. By geometry, QP is parallel to the normal d* (hkl) to the crystal planes and is now 2 sin yðhklÞ 3.5 Scattering by a Crystal Structure 139
- 30. which leads directly to the equation for the structure factor, F. The scattering of X-rays by a crystal comprises two parts: a geometrical part that depends on the symmetry of the arrangement of its components, and a structural part that depends upon both the nature of the atoms or molecules comprising those entities and their relative positions in the unit cell. 3.5.1 Structure Factor Equation We need to express the equation that has been deduced for F in a manner that includes the coordinates of the atoms in the unit cell. It follows from (3.46)–(3.48) that the phase for the jth atom, with respect to the origin, can be represented by 2p(hxj + kyj + lzj). Hence, we use this expression in (3.14) to give the structure factor equation for the hkl reﬂection: F(hklÞ ¼ Xn j¼1 fj;y exp½i2pðhxj þ kyj þ lzjÞ (3.63) The structure factor F(hkl) is a dimensionless scalar quantity and refers to the combined scattering from the n atoms in the unit cell to give the hkl spectrum, or equally to the wave from the (hkl) family of planes, relative to the scattering by a single electron at the origin; see also Sect. 3.2.3. The atomic scattering factor fj,y for the jth atom indicates its dependence on y, an alternative parameter to S in this context. Again, frequently the y dependence of f is not expressed in the formula, although it is implicitly always present. The atomic coordinates in (3.63) are fractional values, Sect. 2.2.3, and so are independent of the size of the unit cell. 3.6 Using the Structure Factor Equation In the next two sections, we explore some of the properties and applications of the structure factor equation that are encountered in practical X-ray crystallography. The trigonometrical relations in Web Appendix WA5 may be helpful in some of the ensuing arguments. 3.6.1 Friedel’s Law Except where anomalous scattering is signiﬁcant, Sect. 7.6, X-ray diffraction spectra form a centro- symmetric array. The diffraction spectra from a crystal may be thought of as an expression of its reciprocal lattice, with each spectrum hkl weighted by the corresponding value of the amplitude jF(hkl)j, or the intensity I(hkl). Friedel’s law expresses the centrosymmetric property as IðhklÞ ¼ Iðh k lÞ or jFðhklÞj ¼ jFðh k lÞj (3.64) within the limits of experimental error, and may be derived as follows. Since the atomic scattering factor is a function of (sin y)/l, it will have the same value for both the hkl and h k l reﬂections. Thus, fy ¼ fÀy, because reﬂections from opposite sides of any plane occur at the same value of the Bragg angle y. 140 3 X-Rays and X-Ray Diffraction
- 31. From (3.63) Fðh k lÞ ¼ Xn j¼1 fj exp½Ài2pðhxj þ kyj þ lzjÞ (3.65) and from Fig. 3.13 FðhklÞ ¼ A0 ðhklÞ þ iB0 ðhklÞFðh k lÞ ¼ A0 ðh k lÞ þ iB0 ðh k lÞ ¼ A0 ðhklÞ À iB0 ðhklÞ (3.66) Hence, the following relations hold: fðhklÞ ¼ Àfðh k lÞjFðhklÞj ¼ jFðh k lÞj ¼ ½A02 ðhklÞ þ B02 ðhklÞ1=2 (3.67) and, since I ¼ jFj2 IðhklÞ ¼ Iðh k lÞ (3.68) which is Friedel’s law. 3.6.2 Structure Factor for a Centrosymmetric Crystal One of the questions that frequently arises at the outset of a crystal structure determination is whether or no the space group is centrosymmetric. In a centrosymmetric structure, with the origin on a center of symmetry, the n atoms in the unit cell lie in related pairs, with coordinates Æ(x, y, z). From (3.18) and (3.19), we write for the two parts of the structure factor equation: A0 ðhklÞ ¼ Xn=2 j¼1 fj½cos 2pðhxj þ kyj þ lzjÞ þ cos 2pðÀhxj À kyj À lzjÞ ¼ 2 Xn=2 j¼1 fj cos 2pðhxj þ kyj þ lzjÞ (3.69) where j ranges over the n/2 atoms in the unit cell not related by the center of symmetry. For B0 (hkl), we write B0 ðhklÞ ¼ Xn=2 j¼1 fj½sin 2pðhxs þ kys þ lzsÞ þ sin 2pðÀhxs À kys À lzsÞ ¼ 0 (3.70) Here, B0 ¼ 0 because sin(Àf) ¼ Àsin(f) for all f, in accord with (3.20). In this case, A0 (hkl) ¼ F(hkl), and f(hkl) can take only the values 0 or p, so that the phase angle attaches itself to jF(hkl)j as a positive or negative sign. Hence, we often speak of the signs, s, of reﬂections in centrosymmetric crystals, so that F(hkl) ¼ s(hkl) jF(hkl)j. Clearly, these results apply only when the origin of the unit cell is taken on 1; in any other setting of the origin in a centrosymmetric space group, there will normally be a non-zero component in B0 (hkl). Centrosymmetric crystals usually present fewer 3.6 Using the Structure Factor Equation 141
- 32. difﬁculties to the structure analyst than do non-centrosymmetric crystals because of the above restriction on the phase angles. 3.7 Limiting Conditions and Systematic Absences We considered limiting conditions brieﬂy in Sect. 2.7.1; here we investigate them more fully through the structure factor equation and show how they are handled in several different example symmetries. An X-ray diffraction pattern can be used to determine the type of unit cell that corresponds to the chosen system of reference axes. From (3.63), it would be an unexpected coincidence for many intensities to be zero. With unit cells having no translational symmetry, the intensity of a reﬂection is not usually zero for any particular combinations of h, k, and l, that is, no limiting conditions apply in such a case. Vanishingly weak intensities may arise for certain reﬂections because of the particular structure under investigation; we call these reﬂections accidental absences, and we shall discuss them further, in Sect. 4.2.3. In centered unit cells or in the presence of other translational symmetry, glide planes and screw axes, reﬂections of certain combinations of h, k, and l are totally absent; we call such unobservable reﬂections systematic absences. 3.7.1 Body-Centered Unit Cell As a ﬁrst example, we know that in a body-centered (I) unit cell, the atoms are related in pairs as x, y, z and 1 2 þ x; 1 2 þ y; 1 2 þ z. Using (3.63), we have FðhklÞ ¼ Xn=2 j¼1 fj exp½i2pðhxj þ kyj þ lzjÞ þ exp½i2pðhxj þ kyj þ lzj þ h=2 þ k=2 þ l=2Þ È É (3.71) The term within the braces {...} may be expressed as exp½i2pðhxj þ kyj þ lzjÞf1 þ exp½i2 pðh þ k þ lÞ=2g. Since h + k + l is integral, f1þ exp½i2pðh þ k þ lÞ=2g ¼ 1 þ cos½2pðh þ k þ lÞ =2 ¼ 2 cos2 ½2pðh þ k þ lÞ=4 ¼ G, where G is a multiplying factor for the reduced structure factor equation in centered unit cells; in the body-centered unit cell G ¼ 2, so that FðhklÞ ¼ 2cos2 ½2pðh þ k þ lÞ=4 Xn=2 j¼1 fj exp½i2pðhxj þ kyj þ lzjÞ (3.72) This equation may be broken down into its two components, A0 (hkl) and B0 (hkl), in the usual way. Further simpliﬁcation is possible: in this example, G takes the value 2 if h + k + l is even, and 0 if h + k + l is odd. Hence, we write the limiting condition that shows which reﬂections are permitted by the geometry of an I unit cell as hkl : h þ k þ l ¼ 2n; n ¼ 0; Æ1; Æ2; . . . The same situation expressed as systematic absences, the condition under which reﬂections are forbidden by the space-group geometry, is hkl : h þ k þ l ¼ 2n þ 1; n ¼ 0; Æ1; Æ2; . . . 142 3 X-Rays and X-Ray Diffraction
- 33. Both terms are in common use, and the reader should distinguish between them. We could have reached the same conclusion from (3.71) more speedily: the expression {1 + exp[i2p(h + k + l)/2]} is equal to 1 + exp(ipn), where n is the sum of the integers h, k, and l, and [1 + exp(ipn)] is 2 or 0 for n even or odd. But it is preferable to highlight the dependence on h, k, and l. Analogous expressions can be derived for any centered unit cell. The G factors for all types of centering have been summarized in Table 3.2. It is evident that where a reﬂection arises in a centered unit cell, the structure factor equation has the same form as that for the corresponding primitive unit cell, but multiplied by the G factor appropriate to the unit cell type. The summation in the reduced structure factor equation is then taken over that fraction of atoms not related by the centering symmetry. In practice, the diffraction pattern is recorded, indices allocated to the spectra and then scrutinized for systematic absences, so as to determine the unit cell type. The reader may care to work through the derivations of F(hkl) for, say, a C and an F unit cell, and determine the limiting conditions for each unit cell type; see also Sect. 3.8. 3.7.2 Screw Axes and Glide Planes As we are concerned in this discussion with the geometry of the unit cell rather than the chemical nature of its contents, it is convenient to introduce the following nomenclature. Let N be the total number of atoms in the unit cell, and let n of them be the number in the asymmetric unit, with the number of asymmetric units being m, so that N ¼ nm. Symbolically, we may write XN j¼1 Xn r¼1 Xm s¼1 where the sum over r refers to the symmetry-independent atoms, and that over s to the symmetry- related species. Thus, the structure factor equation contains two parts that may be considered separately. The sum over m symmetry-related atoms is expressed through the coordinates of a set of general equivalent positions. Thus, ArðhklÞ ¼ Xm s¼1 cos 2pðhxs þ kys þ lzsÞ BrðhklÞ ¼ Xm s¼1 sin 2pðhxs þ kys þ lzsÞ (3.73) Extending to the n atoms in the asymmetric unit, with one such term for each atom, A0 ðhklÞ ¼ Xn r¼1 frArðhklÞ B0 ðhklÞ ¼ Xn r¼1 frBrðhklÞ (3.74) The terms Ar(hkl) and Br(hkl) are independent of the nature and arrangement of the atoms in the asymmetric unit; they are a property of the space-group symmetry and are called geometrical 3.7 Limiting Conditions and Systematic Absences 143
- 34. structure factors. We shall consider some examples taken from the monoclinic and orthorhombic systems, in order to show how glide-plane and screw-axis symmetries give rise to limiting conditions with special classes of reﬂections. For this discussion, the subscript s in (3.73) need not be retained, because all m positions are related to the position x, y, z by symmetry, and in the geometrical structure factors we shall, for simplicity, drop the subscript r. Space Group P21 General equivalent positions: x; y; z; x; 1 2 þ y; z, see Fig. 2.30. Geometrical structure factors: AðhklÞ ¼ cos 2pðhx þ ky þ lzÞ þ cos 2pðÀhx þ ky À lz þ k=2Þ ¼ 2 cos 2pðhx þ lz À k=4Þ cos 2pðky þ k=4Þ (3.75) In a similar way, BðhklÞ ¼ sin 2pðhx þ ky þ lzÞ þ sin 2pðÀhx þ ky À lz þ k=2Þ ¼ 2 cos 2pðhx þ lz À k=4Þ sin 2pðky þ k=4Þ (3.76) Limiting Conditions in P21 Geometrical structure factors enable us to determine limiting conditions, that is, to predict which classes of reﬂections are capable of arising in an X-ray diffraction pattern. If we can show, for given values of h, k, and l, that both A(hkl) and B(hkl) are systematically zero, then F(hkl) will be zero, regardless of the atomic positions. For P21, we can cast (3.75) and (3.76) in the following forms, according to the parity (evenness or oddness) of k. Expanding (3.75), we have (see Web Appendix WA5): AðhklÞ=2 ¼ ½cos 2pðhx þ lzÞ þ cos 2pðk=4Þ þ sin 2pðhx þ lzÞ sin 2pðk=4Þ Â ½cos 2pðkyÞ cos 2pðk=4Þ À sin 2pðkyÞ sin 2pðk=4Þ (3.77) In expanding the right-hand side of (3.77), terms such as cos 2pðhx þ lzÞ cos 2pðk=4Þ sin 2pðkyÞ sin 2pðk=4Þ occur. This particular term is equivalent to 1 2 cos 2pðhx þ lzÞ sin 2pðkyÞ sin 4pðk=4Þ which is zero, because k is an integer. Hence, (3.77) becomes AðhklÞ=2 ¼ ½cos 2pðhx þ lzÞ cos 2pðkyÞcos2 2pðk=4Þ À ½sin 2pðhx þ lzÞ Â sin 2pðkyÞ sin2 2pðk=4Þ (3.78) In a similar manner, we ﬁnd from (3.76) BðhklÞ=2 ¼ ½cos 2pðhx þ lzÞ sin 2pðkyÞ cos2 2pðk=4Þ þ ½sin 2pðhx þ lzÞ Â cos 2pðkyÞ sin2 2pðk=4Þ (3.79) 144 3 X-Rays and X-Ray Diffraction
- 35. Separating for k even and k odd, we obtain k ¼ 2n: AðhklÞ ¼ 2 cos 2pðhx þ lzÞ cos 2pðkyÞ (3.80) BðhklÞ ¼ 2 cos 2pðhx þ lzÞ sin 2pðkyÞ (3.81) k ¼ 2n þ 1: AðhklÞ ¼ À2 sin 2pðhx þ lzÞ sin 2pðkyÞ (3.82) BðhklÞ ¼ 2 sin 2pðhx þ lzÞ cos 2pðkyÞ (3.83) Only one systematic condition can be extracted from these equations: if both h and l are zero, then from (3.82) and (3.83). AðhklÞ ¼ BðhklÞ ¼ 0 In other words, the limiting conditions associated with a 21 axis are hkl None (P unit cell) 0k0 k ¼ 2n The example of the 21 axis has been treated in detail; it shows again how a diffraction record may be used to reveal information about the translational symmetry elements of a space group. We can show how the limiting conditions for a 21 axis arise from a consideration of the Bragg equation. Figure 3.22 is a schematic illustration of a 21 symmetry pattern; the motif represents a structure at a height z, and the structure at a height z after operating on it with the 21 axis. The planes MM0 represent the family (0k0) and NN0 the family (02k,0). Reﬂections of the type (0k0) from MM0 planes are canceled by the reﬂections from the NN0 planes, because their phase change relative to MM0 is 180 . Clearly, this result is not obtained with the 02k,0 reﬂections. Although the ﬁgure illustrates the situation for k ¼ 1, the same argument can be applied to any pair of values k and 2k, where k is an odd integer. Limiting conditions for other screw axes, and in other orientations, can be deduced as above, and the results are summarized in Table 3.3. Notice that pure rotation axes, as in space group P2, do not introduce any limiting conditions. Fig. 3.22 Pattern of a structure containing a 21 screw axis: d(NN0 ) ¼ d (MM0 )/2, so that the MM0 planes are halved by the NN0 family 3.7 Limiting Conditions and Systematic Absences 145
- 36. Centric Zones Centric zones, sometimes loosely termed centrosymmetric zones, are of particular importance in crystal structure determination; see also Sect. 4.2.3. In space group P21 and other space groups of crystal class 2, the h0l reﬂections are of special interest. Among (3.80)—(3.83), only (3.80) is relevant here because zero behaves as an even number, and sin(2pky)k¼0 ¼ 0. Hence, Aðh0lÞ ¼ 2 cos 2pðhx þ lzÞ Bðh0lÞ ¼ 0 (3.84) From (3.20), f(h0l) is either 0 or p; in other words, the [010] zone is centric for this space group. Centric zones occur in the non-centrosymmetric space groups that have symmetry 2 as a subgroup of their point groups; see Sects. 1.4.2 and 2.7.3ff. Space Group Pc General equivalent positions: x, y, z; x; y; 1 2 þ z. Geometrical structure factors: Proceeding as before, we obtain AðhklÞ ¼ 2 cos 2pðhx þ lz þ l=4Þ cos 2pðky À k=4Þ BðhklÞ ¼ 2 sin 2pðhx þ lz þ l=4Þ cos 2pðky À l=4Þ (3.85) If we expand these equations, as with the example for P21, and then separate the terms for l even and l odd, we shall ﬁnd systematic absences only for the h0l reﬂections. Thus, the limiting conditions for Pc are hkl None h0l l ¼ 2n The relationship between the index (l) involved in the condition and the symmetry translation (c/2) is clear. A space group diagram for Pc is shown in Fig. 3.23. Space Group P21/c This space group contains the two translational symmetry operations already discussed, namely, a 21 axis parallel to y and a c-glide normal to y, Fig. 2.32 and Problem 2.8a. It is a centrosymmetric space group, and the general equivalent positions may be summarized as Table 3.3 Limiting conditions for screw axes Screw axis Orientation Limiting condition Translational component 21 k x h00: h ¼ 2n a/2 21 k y 0k0: k ¼ 2n b/2 21 k z 00l: l ¼ 2n c/2 31 or 32 k z 000l: l ¼ 3n c/3 or 2c/3 41 or 43 k z 00l: l ¼ 4n c/4 or 3c/4 42 k z 00l: l ¼ 2n 2c/4 (c/2) 61 or 65 k z 000l: l ¼ 6n c/6 or 5c/6 62 or 64 k z 000l: l ¼ 3n 2c/6 (c/3), c/6(2c/3) 63 k z 000l: l ¼ 2n 3c/6 (c/2) In the cubic system, 41, 43, and 42 axes parallel to x and y exhibit limiting conditions similar to those parallel to z by cyclic permutation 146 3 X-Rays and X-Ray Diffraction
- 37. Æ fx; y; z; x; 1 2 À y; 1 2 þ zg Geometrical structure factors: In the standard setting of this space group, the origin is on 1, so that we can immediately apply (3.69) and (3.70) and write AðhklÞ ¼ 2fcos 2p½hx þ ky þ lz þ cos 2p½hx À ky þ lz þ ðk þ lÞ=2gBðhklÞ ¼ 0 (3.86) Combining the two cosine terms AðhklÞ ¼ 4 cos 2p½hx þ lz þ ðk þ lÞ=4 cos 2p½ky À ðk þ lÞ=4Þ Separating for k + l even and odd, we obtain k þ l ¼ 2n; AðhklÞ ¼ 4 cos 2pðhx þ lzÞ cos 2pðkyÞ k þ l ¼ 2n þ 1; AðhklÞ ¼ À4 sin 2pðhx þ lzÞ sin 2pðkyÞ (3.87) We now deduce the limiting conditions as hkl None h0l l ¼ 2n (c-glide normal to y) 0k0 k ¼ 2n (21 axis k y) These three classes of reﬂections are important in monoclinic reciprocal space, because only with them can we determine the characteristic systematic absences in the space groups within this system. Despite Friedel’s law, the diffraction symmetry reveals the true space group in this example. Figure 3.24 illustrates weighted reciprocal space levels for a monoclinic crystal of space group Pc, P2/c, or P21/c. Fig. 3.23 Space group Pc. (a) Viewed along c. (b) Viewed along b 3.7 Limiting Conditions and Systematic Absences 147
- 38. Space Group Pma2 From the data in Fig. 3.25 we can write down expressions for the geometrical structure factors: AðhklÞ ¼ cos 2pðhx þ ky þ lzÞ þ cos 2pðÀhx À ky þ lzÞ þ cos 2pðÀhx þ ky þ lz þ h=2Þ þ cos 2pðhx À ky þ lz þ h=2Þ (3.88) Combining the ﬁrst and third, and second and fourth terms, we have AðhklÞ ¼ 2 cos 2pðky þ lz þ h=4Þ þ cos 2pðhx À h=4Þ þ 2 cos 2pðÀky þ lz þ h=4Þ Â cos 2pðhx þ h=4Þ (3.89) Further simpliﬁcation of this expression requires the separate parts to contain a common factor. We return to (3.88) and make a minor alteration to the term cos 2p(hx À ky + lz + h/2). Since h is an integer,we maywrite this termas thecrystallographically equivalentterm cos2p(hx À ky + lz À h/2). Another way of looking at this process is that the fourth general equivalent position has been changed to À 1 2 þ x; y; z, which is equivalent to moving through one repeat a in the negative direction to a crystallographically equivalent position, a perfectly valid and generally applicable tactic. Returning to Pma2, (3.89) now becomes AðhklÞ ¼ 2 cos 2pðky þ lz þ h=4Þ cos 2pðhx À h=4Þ þ 2 cos 2pðÀky þ lz À h=4Þ cos 2pðhx À h=4Þ (3.90) which simpliﬁes to AðhklÞ ¼ ½2 cos 2pðhx À h=4Þ½cos 2pðky þ lz þ h=4Þ þ cos 2pðÀky þ lz À h=4Þ (3.91) Fig. 3.24 Reciprocal nets in the x* , z* plane appropriate to space groups Pc, P2/c, and P21/c. (a) k ¼ 0 and (b) k 0. The c-glide plane, which is perpendicular to b, causes a halving of the rows parallel to x* when k ¼ 0, so that only the rows with l ¼ 2n are present. Hence, the true c* spacing is not observed on the reciprocal lattice level k ¼ 0, but can be determined from higher levels. The symmetry on both levels is 2, in accordance with the diffraction symmetry 2/m: jFðhklÞj ¼ jFðh k lÞj. The reciprocal lattice points are weighted according to jF(hkl)j, or to jF(hkl)j2 , and we speak of such diffraction patterns as weighted reciprocal lattices 148 3 X-Rays and X-Ray Diffraction
- 39. Combining again: AðhklÞ ¼ 4½cos 2pðhx À h=4Þ cos 2pðky þ h=4Þ cos 2plz (3.92) Similarly, BðhklÞ ¼ 4½cos 2pðhx À h=4Þ cos 2pðky þ h=4Þ sin 2plz (3.93) In the orthorhombic system, seven regions of reciprocal space of particular importance are listed on the right-hand side of Fig. 3.25. Separating (3.92) and (3.93) for even and odd values of h, we obtain h ¼ 2n : AðhklÞ ¼ 4 cos 2phx cos 2pky cos 2plz BðhklÞ ¼ 2 cos 2phx cos 2pky sin 2plz (3.94) h ¼ 2n þ 1 : AðhklÞ ¼ À4 sin 2phx sin 2pky cos 2plz BðhklÞ ¼ À4 sin 2phx sin 2pky sin 2plz (3.95) from which we ﬁnd the limiting conditions hkl None h0l h ¼ 2n Fig. 3.25 General equivalent positions and symmetry elements in space group Pma2, with the origin on 2; the origin is not ﬁxed in the z direction by the symmetry elements. The diagram shows inter alia the coordinates of the special equivalent positions and the limiting conditions 3.7 Limiting Conditions and Systematic Absences 149
- 40. The listed condition h00: (h ¼ 2n) should be considered carefully. One might be excused for thinking at ﬁrst that it implies the existence of a 21 axis parallel to the x axis, but for the knowledge that there are no symmetry axes parallel to the x axis in class mm2. This particular limiting condition is dependent upon the h0l condition: h00 is in the h0l zone. We emphasize here that confusion can very easily arise if the limiting conditions are interpreted in other than the following hierarchal order: Order of inspection Downward hkl Unit cell type #0kl Glide plane ⊥x h0l Glide plane ⊥y hk0 Glide plane ⊥z h00 21 axis jj x 0k0 21 axis jj y 00l 21 axis jj z One should proceed to a lower level in this list only after considering the full implications of the conditions at higher levels. Conditions such as that for h00 in Pma2 are called redundant or dependent and are placed in parentheses on the diagram. Reﬂections involved in such conditions are certainly absent from a diffraction record, but do not contribute to the determination of space-group symmetry. Table 3.4 summarizes the limiting conditions for glide-plane symmetry. Space Group Pman This space group may be derived from Pma2 by the addition of an n-glide plane perpendicular to the z axis, with a translational component of (a + b)/2. We have now seen on several occasions that it is advantageous to set the origin at 1 wherever possible; Fig. 3.26 shows Pman drawn in this orientation. It is left to the reader to show that the geometrical structure factors are AðhklÞ ¼ 8 cos 2phx cos 2p½ky À ðh þ kÞ=4 cos 2p½lz þ ðh þ kÞ=4 BðhklÞ ¼ 0 (3.96) and subsequently to derive the limiting conditions for this space group. Table 3.4 Limiting conditions for glide planes Glide plane Orientation Limiting condition Translational component a ⊥b h0l: h ¼ 2n a/2 a ⊥c hk0: h ¼ 2n a/2 b ⊥a 0kl: k ¼ 2n b/2 b ⊥c hk0: k ¼ 2n b/2 c ⊥a 0kl: l ¼ 2n c/2 c ⊥b h0l: l ¼ 2n c/2 n ⊥a 0kl: k + l ¼ 2n (b + c)/2 n ⊥b h0l: l + h ¼ 2n (c + a)/2 n ⊥c hk0: h + k ¼ 2n (a + b)/2 d ⊥a 0kl: k + l ¼ 4n (k, l ¼ 2n) (b Æ c)/4 d ⊥b h0l: l + h ¼ 4n (l, h ¼ 2n) (c Æ a)/4 d ⊥c hk0: h + k ¼ 4n (h, k ¼ 2n) (a Æ b)/4 150 3 X-Rays and X-Ray Diffraction
- 41. Space Group P63 ⁄m Finally here, and in order to show that these manipulations are fundamentally no more difﬁcult with a space group not based on orthogonal axes, we study the hexagonal space group P63/m; we will address the tetragonal system through space group P4nc in a problem. From Fig. 2.38, we list the coordinates as: Æ fx; y; z; y; x À y; z; x þ y; x; z; x; y; 1 2 þ z; y; x þ y; 1 2 þ z; x À y; x; 1 2 þ zg Fig. 3.26 Space group Pman. (a) General equivalent positions. (b) Symmetry elements; the origin is on 1. The diagram shows also the limiting conditions for this space group. 3.7 Limiting Conditions and Systematic Absences 151
- 42. Since the structure is centrosymmetric, with the origin on 6/m ð1Þ, we need consider only the cosine part of the structure factor equation (B ¼ 0). Thus, following (3.69) we can write the geometrical structure factor as: A=2 ¼ cos 2pðhx þ ky þ lzÞ þ cos 2pðÀhy þ k½x À y þ lzÞ þ cos 2pðh½ y À x À kx þ lzÞ þ cos 2pðÀhx À ky þ lz þ l=2Þ þ cos 2pðhy þ k½ y À x þ lz þ l=2Þ þ cos 2pðh½x À y þ kx þ lz þ l=2Þ Combining the cosine terms in pairs, we obtain A=4 ¼ cos 2pðlz À l=4Þfcos 2pðhx þ ky þ l=4Þ þ cos 2pðkx þ iy þ l=4Þ þ cos 2pðix þ hy þ l=4Þg [remember that i ¼ À(h + k)]. We can now separate into equations for l even and l odd by expanding the cosine terms (you may need Web Appendix WA5): l ¼ 2n: A ¼ 4 cos 2plzfcos 2pðhx þ kyÞ þ cos 2pðkx þ iyÞ þ cos 2pðix þ hyÞg l ¼ 2n þ 1: A ¼ À4 sin 2plzfsin 2pðhx þ kyÞ þ sin 2pðkx þ iyÞ þ sin 2pðix þ hyÞg For l even, there are no reﬂection conditions; for l odd, A ¼ 0 if h ¼ k ¼ 0. Thus, the only condition limiting X-ray reﬂections is 000l ¼ l ¼ 2n. The expression above for A/2 differs in a trivial manner from that given in the International Tables [10]: the value therein may be achieved by using initially the crystallographically equivalent position ðÀ 1 2 þ zÞ, in place of the 1 2 þ z employed here. 3.8 Practical Determination of Space Groups from Diffraction Data The determination of the space group of a crystal is an important and early feature in the X-ray analysis of its structure. We shall assume that we have available the X-ray diffraction record for the several examples of monoclinic and orthorhombic crystals to be examined. It is necessary to bear in mind that X-ray techniques can reveal the presence of that translational symmetry which can arise through symmetry operations: 1. Translations relating to centering of the unit cell (a/2 and/or b/2 and/or c/2). 2. Translations relating to glide planes. 3. Translations relating to screw axes. or any combination of these symmetry operations. All categories lead to systematic absences, and the totality of the translational symmetry, together with the Laue group, forms the diffraction symbol, Sect. 2.9. 152 3 X-Rays and X-Ray Diffraction
- 43. 3.8.1 Monoclinic Space Groups Single crystal X-ray photographs taken with a monoclinic crystal showed typically the reﬂections listed in Table 3.5. From the important reﬂection types, hkl, h0l, and 0k0, we deduce the limiting conditions: hkl h + k ¼ 2n h0l (h ¼ 2n) 0k0 (k ¼ 2n) Using Table 3.7, we conclude that for crystal I, the space group is one of C2, Cm, or C2/m. The diffraction data alone do not distinguish between these three possible space groups; we show in Sect. 4.2.3ff how this ambiguity might be resolved. Table 3.6, for monoclinic crystal II, provides the next list of diffraction data for inspection. Table 3.5 Some reflection data for monoclinic crystal I hkl 200 401 112 510 201 402 113 020 202 600 114 040 203 110 310 060 400 111 311 080 Table 3.6 Some reflection data for monoclinic crystal II hkl 100 204 111 322 200 402 122 020 300 502 113 040 400 110 311 060 202 310 123 080 Table 3.7 Limiting conditions for the mono- clinic space groups Conditions limiting possible X-ray reﬂections Space groups hkl: none h0l: none 0k0: none ) P2, Pm, P2/m hkl: none h0l: none 0k0: k ¼ 2n ) P21, P21/m hkl: none h0l: l ¼ 2n 0k0: none ) Pc, P2/c hkl: none h0l: l ¼ 2n 0k0: k ¼ 2n ) P21/c hkl: h þ k ¼ 2n h0l: none 0k0: none ) C2, Cm, C2/m hkl: h þ k ¼ 2n h0l: l ¼ 2nðh ¼ 2nÞ 0k0: none ) Cc, C2/c 3.8 Practical Determination of Space Groups from Diffraction Data 153
- 44. There is no condition on hkl, but h0l are restricted by l being even, and 0k0 by k being even: this space group is identiﬁed uniquely as P21/c. The limiting conditions for the 13 monoclinic space groups are listed in Table 3.7, in their standard orientations. In practice, it is possible, by an inadvertent choice of axes, to ﬁnd oneself working with a non-standard space-group symbol. Generally, a fairly straightforward transformation of axes will lead to the standard setting (see Problems 2.12 and 3.17). 3.8.2 Orthorhombic Space Groups We begin with the sample data in Table 3.8. From these data, we deduce the conditions below: Limiting conditions deduced: hkl None h00 h ¼ 2n 0kl None 0k0 k ¼ 2n h0l None 00l l ¼ 2n hk0 None Examining in the prescribed hierarchy, we ﬁnd only 21 axes parallel to x, y, and z: the space group is determined uniquely as P212121, Sect. 2.7.7 and Table 2.7. In the ﬁnal two examples, we consider only the conclusions drawn from an inspection of the diffraction records. In the ﬁrst instance, we have: hkl None h00 None 0kl k ¼ 2n 0k0 (k ¼ 2n) h0l l ¼ 2n 00l (l ¼ 2n) hk0 None The diffraction symbol is mmm PbcÃ so that the space group is either Pbc21 or Pbcm; the distinction between them depends upon the presence, or otherwise, of a center of symmetry. In the second example, we have: hkl None h00 (h ¼ 2n) 0kl k ¼ 2n 0k0 (k ¼ 2n) h0l l ¼ 2n 00l (l ¼ 2n) hk0 h ¼ 2n and space group Pbca is uniquely determined. These results seem quite reasonable and straightforward, but nevertheless, one might be tempted to question their validity. For example, in the ﬁrst orthorhombic crystal, is there a space group in class mmm that would give the same systematic absences as those in Table 3.8? Experience tells us that there is not. Since no glide planes are indicated by the systematic absences, the three symmetry planes, if present, would have to be m-planes. Three m-planes could not be involved with three 21 Table 3.8 Some reflection data for an ortho- rhombic crystal hkl 111 011 110 020 112 021 120 040 212 012 310 060 312 101 200 002 322 203 400 004 332 303 600 006 154 3 X-Rays and X-Ray Diffraction
- 45. axes unless the unit cell were centered, for example, as in Immm, which would restrict the hkl reﬂections to h + k + l ¼ 2n. Hence, our original conclusion is correct. 3.8.3 Tetragonal Space Groups The following reﬂections conditions were obtained for two tetragonal crystals of Laue groups 4 m mm and 4 m , respectively. It may help to consider again Table 1.5. (a) hkl : none hk0 : h þ k ¼ 2n 0kl : k ¼ 2n P n ? z b ? x Consulting the International Tables, Volume 1 (or Volume A) on diffraction symbols shows that this space group is P 4 n bm. (b) hkl : h þ k þ l ¼ 2n hk0 : h; ðkÞ ¼ 2n 00l : l ¼ 4n I a ? z 41 jj z This space group is I 41 a . 3.8.4 Hexagonal Space Groups The following reﬂections conditions were obtained for two hexagonal crystals of point groups (a) 622 and (b) either 6 m mm or 6mm, respectively. (a) hkil : none 000l : l ¼ 6n P 61 or 65 The diffraction symbol is: 622 P 61ð65Þ Ã Ã; thus, the space group is either P6122 or its enantio- morph P6522. (b) hkl : none h0hl : l ¼ 2n P c?x; ðyÞ If the point group is 6 m mm, reference to the International Tables for diffraction symbol 6 m mmPÃcÃ leads to the space group is P 63 m cm, whereas if the point group is 6mm, similar considerations indicate space group P63cm. The practicing X-ray crystallographer is assisted by the information on space groups in Volume A (and the earlier Volume 1) of the International Tables for Crystallography [10]. Combined with a working knowledge of symmetry, these tables enable most symmetry situations arising in the course of a structure analysis to be treated correctly. 3.9 Problems 3.1. What is the change in wavelength of an X-ray photon scattered incoherently by a free electron at 45 to the forward direction of the incident beam? If the wavelength of the incident photon is 1 A˚ , what is the energy of the scattered photon? 3.9 Problems 155
- 46. 3.2. Two identical coherent scattering centers are separated by the distance 2l, and X-rays fall normally on to the line joining the two centers. For 2y ¼ 0 to 180 in steps of 30 , calculate the scattered amplitudes and intensities as fractions of the results with both scatterers at one point. 3.3. Calculate the atomic scattering factor f for beryllium at (sin y)/l ¼ 0.0, 0.2, and 0.5. The expression for f(1s) has been given in the text. The Slater wave function for the 2s electron may be given as C2s ¼ ðc5 2= 96pÞ1=2 r expðc2r=2Þ; you may need the general result Ð1 0 xn expðÀaxÞ sin bx dx ¼ n!½ða þ ibÞnþ1 Àða À ibÞnþ1 =½2iða2 þ b2 Þnþ1 , from which the similar expression given in the text for the 1s wavefunction applies for the case n ¼ 1. The screening constants for beryllium are s1s ¼ 0.3 and s2s ¼ 2.05. Compare the results that are obtained for f with those from the expression f ¼ P4 j aj expðÀbjs2 Þ þ c, where s is (sin y)/l and the values of a, b, and c for beryllium are listed below: a1 b1 a2 b2 a3 b3 a4 b4 c 1.5919 43.6427 1.1278 1.8623 0.5391 103.483 0.7029 0.5420 0.0385 3.4. An X-ray tube is operated at 30 kV. What is the energy, in J, associated with each X-ray photon produced by the tube? 3.5. Calculate the transmittance factor (I/I0) for a 1 mm crystal plate of benzene (C6H6), the density of which is 1,124 kg mÀ3 . The mass absorption coefﬁcient for Cu Ka X-radiation and the relative atomic masses are as follow: C H m/m2 kgÀ1 0.46 0.04 Mr 12.01 1.008 3.6. There are eight combinations of one to three negative signs among the indices hkl for any general reﬂection. With the aid of the geometrical structure factors given in the text, derive the relationships between the eight forms of the phase angle f(hkl) for (a) space group P21 and (b) space group Pma2. 3.7. A triclinic unit cell has the dimensions a ¼ 7.36 A˚ , b ¼ 9.21 A˚ , c ¼ 13.47 A˚ , and a ¼ 101.22 , b ¼ 110.62 , g ¼ 123.41 . Calculate (a) the six parameters of the reciprocal unit cell for Cu Ka radiation (l ¼ 1.5418 A˚ ), and (b) the volumes of the real and reciprocal unit cells. 3.8. In the direct unit cell of Problem 3.7, two atoms are situated at the fractional coordinates 0.10, 0.30, 0.20 and 0.10, 0.15, 0.35 for x, y, z, respectively. By means of vector expressions, calculate the distance between the two atoms, and the angle subtended at the origin by the vectors from the origin to each of the two atoms. 3.9. Three atoms have the following amplitudes and phases with respect to the real axis of an Argand diagram: (a) 13.1, 16.23 (b) 21.4, 154.87 (c) 37.9, À113.26 Calculate the amplitude and phase of the resultant sum. 3.10. Express the structure factor equation in a reduced form for an A-face centered unit cell. Hence, deduce the limiting conditions associated with A centering. 156 3 X-Rays and X-Ray Diffraction
- 47. 3.11. A two-dimensional structure has four atoms per unit cell, two of type P and two of type Q, with the following fractional coordinates: x y P1 0.1 0.2 P2 0.9 0.8 Q1 0.2 0.7 Q2 0.8 0.3 Calculate jF(hk)j for the reﬂections 5 0, 0 5, 5 5 and 5 10 in terms of the scattering factors gP and gQ for the two species. If gP ¼ 2gQ, what are the phase angles for these reﬂections? 3.12. a-Uranium crystallizes in the orthorhombic system with four uranium atoms in special positions: Æ f0; y; 1 4; 1 2; 1 2 þ y; 1 4g Use the data below to decide whether y is better chosen as 0.10 or 0.15. hkl jF(hkl)j gU(hkl) 020 88.5 70.0 110 268.9 80.0 3.13. The unit cell dimensions of a-uranium are a ¼ 2.85 A˚ , b ¼ 5.87 A˚ , c ¼ 5.00 A˚ . Use the value of yU from Problem 3.12 to determine the shortest U–U distance in the structure. It may be helpful to plot the uranium atom positions in a few neighboring unit cells. 3.14. In the examples listed below for monoclinic crystals, the conditions limiting possible X-ray reﬂections are given. In each case, write the possible space groups corresponding to the information given. (a) hkl None h0l None 0k0 k ¼ 2n (b) hkl None h0l h ¼ 2n 0k0 None (c) hkl h + k ¼ 2n h0l l ¼ 2n (h ¼ 2n) 0k0 (k ¼ 2n) (d) hkl None h0l None 0k0 None 3.9 Problems 157
- 48. 3.15. Repeat Problem 3.14, but for the limiting conditions below relating to orthorhombic crystals. (a) hkl None h00 h ¼ 2n 0kl None 0k0 k ¼ 2n h0l None 00l None hk0 None (b) hkl None h00 None 0kl k ¼ 2n 0k0 k ¼ 2n h0l None 00l None hk0 None (c) hkl h + k + l ¼ 2n h00 h ¼ 2n 0kl k ¼ 2n, l ¼ 2n 0k0 k ¼ 2n h0l h + l ¼ 2n 00l l ¼ 2n hk0 h + k ¼ 2n 3.16. (a) Write the independent conditions limiting possible X-ray reﬂections for the following space groups: (i) P21/a; (ii) Pc; (iii) C2; (iv) P2122; (v) Pcc2; (vi) Imam. In each case, write the symbols of the space groups, if any, in the same crystal system with the same limiting conditions. (b) Write the conditions limiting possible X-ray reﬂections in the monoclinic space group P21/n (non-standard setting). (c) Give the conventional symbols for the space groups A2/a and B21221. 3.17. (a) Space group Pcab corresponds to the non-standard setting acb, that is, a along x, Àc along y, and b along z. What is the symbol in the standard (abc) setting? (b) What is the essential difference between the space groups represented by the standard symbols Pmna and Pnma? What are their full symbols? 3.18. The absorption correction for a crystal ground into a sphere of radius r is dependent on r, m, and y. Assume that extinction effects are negligible and determine the ideal intensity for an hkl reﬂection, given that the measured intensity less background is 56.3, and that r ¼ 0.11 mm and m ¼ 18.2 Â 103 mÀ1 . For this reﬂection, y ¼ 30 , and some tabulated data are listed above, corresponding to the numerical integration A ¼ fð1=VÞ Ð dx Ð dy Ð exp½Àm ðr0 þ rÞ dzgÀ1 , where r0 and r are, respectively, the incident and diffracted paths lengths in the crystal. Include the y-dependent Lorentz and polarization corrections. Transmission factors A for a sphere of radius R and linear absorption coefficient y/ mR 25 30 35 1 3.88 3.79 3.70 2 10.9 10.0 9.26 3 22.4 19.5 17.1 4 37.2 31.0 26.3 158 3 X-Rays and X-Ray Diffraction
- 49. 3.19. For space group P63/m, what are (a) the Sch€onﬂies point group symbol, (b) the full Hermann–Mauguin point-group and space-group symbols, (c) the crystal system, (d) the crystal class, (e) the lattice, and (f) the conventional unit cell? 3.20. Using the coordinates of the general equivalent positions for space group P4nc, Fig. 2.37, derive (a) the geometrical structure factors, (b) the amplitude symmetry, (c) the phase-angle symmetry. References 1. See Bibliography, International tables for X-ray crystallography, vol 4 2. Gilfrich JV et al (1995) Advances in X-ray analysis, vol 39. In: Proceedings of the 45th annual conference on applications of X-ray analysis, Colorado Springs 3. http://blog.the-scientist.com/2011/04/11/multipole-wigglers/ 4. Karsch S et al (2010) Max-Planck Instit€ut f€ur Quantenoptik. In: Osterhoff Jens (ed) Laser-plasma acceleration. Universit€at Hamburg, Hamburg 5. See Bibliography: James (1958), Woolfson (1977) or http://www.gwyndafevans.co.uk/thesis-html/node11.html 6. Ladd M (1998) Introduction to physical chemistry, 3rd edn. Cambridge University Press, Cambridge 7. (1962) International tables for X-ray crystallography, vol IV. Kynoch Press 8. Ewald PP (1913) Z Phys 14:465 9. Holmes KC (2006) Nature 440:149 10. See Bibliography, Chapter 1, Henry et al (1965) Bibliography: Synchrotron Radiation Helliwell JR (1992) Macromolecular crystallography with synchrotron radiation. Cambridge University Press, Cambridge Structure Factor and Intensity James RW (1958) Optical principles of the diffraction of X-rays: the crystalline state, vol 2. Bell, London Prince E, Wilson AJC (1999) International tables for X-ray crystallography, vol C, 2nd edn. Kluwer Academic, Dordrecht Woolfson MM (1977) An introduction to X-ray crystallography, 2nd edn. Cambridge University Press, Cambridge Atomic Scattering Factors Ibers JA, Hamilton WC (eds) (1974) International tables for X-ray crystallography, vol 4. Kynoch Press, Birmingham References 159

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment